Upcoming SlideShare
×

# Manual

188

Published on

Published in: Education
0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total Views
188
On Slideshare
0
From Embeds
0
Number of Embeds
0
Actions
Shares
0
6
0
Likes
0
Embeds 0
No embeds

No notes for slide

### Transcript of "Manual"

1. 1. 1  ___________________________________________  Strength of materials  Lab. Manual ______________________________________________________________________________________________  Production Engineering
2. 2. 2  Strength of materials lab. manual  _________________________________________________________________  Contents ___________________________________________________________________  S.No.                  Title  Pg.no  _________________________________________________________________  1.                    Rockwell Hardness test                     3  2.                    Brinell hardness test.                         5  3.                    Impact test  8  4.                    Tension test                                       14  5.                    Torsion test                                        19  6.                    Bending test  21  7.                    Shear test                                           24  8.                    Compression test                              26  ________________________________________________________________  Instructions.­1.Write  observations,  tables,  diagrams,  Specimen  calculations  in the blank left side of the journal and others to the right.
4. 4. 4  5.  Repeat the procedure five times on the specimen selecting different points for  indentation.  Observation  1.  Take  average  of  five  values  of  indentation  of  each  specimen.  Obtain  the  hardness number from the dial of a machine.  2.  Compare Brinell and Rockwell hardness tests obtained.  Figure .1  Rockwell hardness test equipment  Result  Rockwell hardness of given specimen is ­­­­­­­­­
5. 5. 5 Experiment No.2 ________________________________________________________________ Title  Brinell hardness test. Aim  To determine the hardness of the given specimen using Brinell hardness  test. Specimen and specimen  Brinell hardness tester (fig.2)  Aluminum specimen  Ball indenter. Precautions 1.  Thickness  of  the  specimen  should  not  be  less  than  8  times  the  depth  of  indentation to avoid the deformation to be extended to the opposite surface of  a specimen. 2.  Indentation  should  not  be  made  nearer  to  the  edge  of  a  specimen  to  avoid  unnecessary concentration of stresses. In such case distance from the edge to  the  center  of  indentation  should  be  greater  than  2.5  times  diameter  of  indentation. 3.  Rapid  rate  of  applying  load  should  be avoided.  Load applied on  the ball  may  rise  a  little  because of  its sudden  action.  Also  rapidly  applied  load will  restrict  plastic flow of a material, which produces effect on size of indentation. 4.  Surface of the specimen is well polished, free from oxide scale and any foreign  material. Theory Hardness  of  a  material  is  generally  defined  as  Resistance  to  the  permanent indentation  under  static  and  dynamic  load.  When  a  material  is  required  to  use under direct static or dynamic loads, only indentation hardness test will be useful to find out resistance to indentation. In Brinell hardness test, a steel ball of diameter (D) is forced under a load (F) on to a surface of test specimen. Mean diameter (d) of indentation is measured after the removal of the load (F). Observation  1.  Take  average  of  five  values  of  indentation  of  each  specimen.  Obtain  the  hardness number from equation (!).  2.  Compare Brinell and Rockwell hardness tests obtained. Procedure
6. 6. 6 1.Load  to  be  applied  for  hardness  test  should  be  selected  according  to  the expected  hardness  of  the  material.    However  test  load  shall  be kept  equal  to  30 times the square of the diameter of the ball (diameter in mm)  2 F=30.D Where ball diameter, generally taken as 10 mm.  For guidelines hardness range for standard loads given below  Ball diameter  Load (kg)  Range of Brinell hardness  10  3000  96 to 600  1500  48 to 300  500  16 to 100 2.Apply  the  load  for  a  minimum  of  15  seconds  to  30  seconds.  [if  ferrous metals  are  to  be  tested  time  applied  will  be  15  seconds  and  for  softer  metal  30 seconds] 3.Remove the load and measure the diameter of indentation nearest to 0.02 mm using microscope (projected image) 4.Calculate Brinell hardness number (HB). As per IS: 1500. 5.Brinell hardness number 2  F (1)  [p D  D  - D  2  - d  2  ] where D is the diameter of ball indenter and d is the diameter of indentation. Hardness  numbers  normally  obtained  for  different  materials  are  given  below (under 3000 kg and 10 mm diameter ball used)  Ordinary  steels  medium  100 to 500  carbon  130 to 160  Structural steel  800 to 900  Very hard steel Note:  Brinell test is not recommended for then materials having HB over 630. It is necessary to mention ball size and load with the hardness test when standard size  of ball and  load  are  not  used.  Because indentation  done  by  different size of ball  and  load  on  different  materials  are  not  geometrically  similar.  Ball  also
7. 7. 7 undergoes deformation when load is applied. Material response to the load is not same all the time. 6.Brinell hardness numbers can be obtained from tables 1 to 5 given in IS: 1500, knowing diameter of   indentation, diameter of the ball and load applied. Figure 2  Brinell hardness tester Result; The Brinell hardness number of the specimen is ­­­­­­­
8. 8. 8  Experiment No.3 _______________________________________________________________________  Title         Impact test  Aim  To determine the Impact toughness (strain energy) through  Izod test and Charpy test  Theory  In  a  impact  test  a  specially  prepared  notched  specimen  is  fractured  by  a  single  blow from a heavy hammer and energy required being a measure of resistance to  impact.  Impact  load  is  produced  by  a  swinging  of  an  impact  weight  W  (hammer)  from  a  height h. Release of the weight from the height h swings the weight through the arc  of a circle, which strikes the specimen to fracture at the notch (fig..  2  Kinetic energy of the hammer at the time of impact is mv  /2, which is equal to the  relative  potential  energy  of  the  hammer  before  its  release.  (mgh),where  m  is  the  mass  of  the  hammer  and  v  = 2 gh  is  its  tangential  velocity  at  impact,  g  is  2  gravitational  acceleration  (9.806  m/s  )  and  h  is  the  height  through  which  hammer  falls. Impact velocity will be 5.126 m/s or slightly less.  Here  it  is  interesting  to  note  that  height  through  which  hammer  drops  determines  the velocity and height and mass of a hammer combined determine the energy.  Energy  used  can  be  measured  from  the  scale  given.  The  difference  between  potential  energies  is  the  fracture energy.    In  test  machine  this  value  indicated  by  the  pointer  on  the  scale.  If  the  scale  is  calibrated  in  energy  units,  marks  on  the  scale should be drawn keeping in view angle of fall () and angle of rise (. Height h1  and h2  equals,  h1= R (1­cos q) and h2= (1­cos q).  With  the  increase  or  decrease  in  values,  gap  between  marks  on  scale  showing  energy also  increase or decrease.  This can be seen from the attached scale  with  any impact machine.  Energy used in fracturing the specimen can be obtained approximately as  Wh1­Wh2  This  energy  value  called  impact  toughness  or  impact  value,  which  will  be  measured, per unit area at the notch.  Izod introduced Izod test in 1903. Test is as per the IS: 1598  Charpy introduced Charpy test in 1909. Test is as per the IS: 1499.
9. 9. 9  a. Izod test Specimen and equipment 1.  Impact testing machine.(fig.3) 2.  Specimen and v notch is shown in the fig.4. Size of the specimen is 10mm  X 10mm X 75mm Mounting of the specimen: Specimen  is  clamped  to  act  as  vertical  cantilever  with  the  notch  on  tension side. Direction of blow of hammer is shown in fig. (). Direction of blow is shown in fig Figure. 3.a  Izod Impact testing equipment
10. 10. 10  Figure 3.b  Schematic impact testing Figure 4  Position of specimen for Izod test
11. 11. 11 Procedure 1.  Measure the dimensions of a specimen. Also, measure the dimensions of  The notch. 2.  Raise the hammer and note down initial reading from the dial, which will be  energy to be used to fracture the specimen. 3.  Place the specimen for test and see that it is placed center with respect to  hammer. Check the position of notch. 4.  Release the hammer and note the final reading. Difference between the  initial and final reading will give the actual energy required to fracture the  Specimen. 5.  Repeat the test for specimens of other materials. 6.  Compute the energy of rupture of each specimen. Observation  Initial and final reading of the dial. Result  Strain energy of given specimen is ­­­­­­­­­  b.  Charpy test Specimen and equipment: 1.  Impact testing machine. (Fig.6) 2.  U notch is cut across the middle of one face as shown in (fig.5). Figure 5  Specimen for Charpy test
12. 12. 12 Figure 6  Charpy impact testing equipment Mounting of specimen Specimen is tested as a beam supported at each end (fig.7). Hammer is allowed to hit then specimen at the opposite face behind the notch. Figure.7  Mounting of specimen
13. 13. 13  Procedure 1.  Measure the dimensions of a specimen. Also, measure the dimensions of  The notch. 2.  Raise the hammer and note down initial reading from the dial, which will be  energy to be used to fracture the specimen. 3.  Place the specimen for test and see that it is placed center with respect to  hammer. Check the position of notch. 4.  Release the hammer and note the final reading. Difference between the  initial and final reading will give the actual energy required to fracture the  Specimen. 5.  Repeat the test for specimens of other materials. 6.  Compute the energy of rupture of each specimen.  Observation  Initial and final reading of the dial.  Result  Strain energy of given specimen is ­­­­­­­­­
14. 14. 14 Experiment No.4 __________________________________________________________________ Title:  Tension test Aim:                 To determine the tensile strength of specimen Specimen and equipments  Universal testing machine (fig7.a)  Specimen as shown in the( fig7.b)  Of different ferrous and non ferrous materials Figure 7.a